# thermal diffusivity and thermal conductivity by diffusivity and thermal conductivity by lfa ......

Post on 03-May-2018

223 views

Category:

## Documents

Embed Size (px)

TRANSCRIPT

• www.netzsch.com

Analyzing & Testing

LFA for Thermal Diffusivity and Conductivity of

Metals, Ceramics and Polymers

Ramn Arauz Lombardia, Service & Applications

NETZSCH-Gertebau GmbH, Branch Office Barcelona, Spain

• www.netzsch.com Thermal Diffusivity and Thermal Conductivity by LFA 1

Agenda

1. Heat Transfer - Basics

2. LFA - Method

3. LFA - Instrumentation

4. Application Examples

5. Summary

• www.netzsch.com Thermal Diffusivity and Thermal Conductivity by LFA 2 2

Examples of Heat Transfer

From Everyday Life

..cooling the microprocessor chip in a laptop computer

2

Heat Transfer Electronics

• www.netzsch.com Thermal Diffusivity and Thermal Conductivity by LFA 3 3

Examples of Heat Transfer

From Everyday Life

3

Photo: BMW AG Photo-Gallery: 3 Series

Thermal Conductivity Automotive Industry

• www.netzsch.com Thermal Diffusivity and Thermal Conductivity by LFA 4 4

Heat Transfer - Basics

4

x

Tq

x

TTAQ

;12

Heat transfer (or heat) is the energy in transit (energy moving

through a material) due to a temperature difference.

A quantitative expression relating the rate of heat transfer, the

temperature gradient and the nature of the conducting medium is

attributed to Fourier (1822):

Jean Baptiste Joseph Fourier

Heat flux = heat

flow rate per unit

area in direction x

- thermal

conductivity

of material

A area normal to heat flow

• www.netzsch.com Thermal Diffusivity and Thermal Conductivity by LFA 5 5

Heat Transfer - Basics

There are three main modes of heat transfer:

Conduction: molecular interactions or free electrons

Convection: exchange of heat between a fluid and a surface or an

interface.

Radiation: no medium required, electromagnetic phenomenon

Stefan-Boltzmann constant

Thermal conductance varies for each mode of heat transfer

5

4TA

q

• www.netzsch.com Thermal Diffusivity and Thermal Conductivity by LFA 6 6

Heat Transfer Basics

6

• www.netzsch.com Thermal Diffusivity and Thermal Conductivity by LFA 7 7

Thermal Conductivity Measurement Methods

7

• www.netzsch.com Thermal Diffusivity and Thermal Conductivity by LFA 8

Agenda

1. Heat Transfer - Basics

2. LFA - Method

3. LFA - Instrumentation

4. Application Examples

5. Summary

• www.netzsch.com Thermal Diffusivity and Thermal Conductivity by LFA 9 9

Heat Transfer LFA Method

9

The measurement of the thermal diffusivity of a material is usually carried out

by rapidly heating one side of a sample and measuring the temperature rise

curve on the opposite side.

The time that it takes for the heat to travel through the sample and cause the

temperature to rise on the rear face can be used to measure the through-plane

diffusivity and calculate the through-plane thermal conductivity if the specific heat

and density are known.

All three quantities as well as the thermal diffusivity can be functions of

temperature.

TTcTaT p

• www.netzsch.com Thermal Diffusivity and Thermal Conductivity by LFA 10 10

Heat Transfer LFA Method

10

Flash Method:

Measurement Principle

Introduced by Parker et al. 1961

The front surface of a plan-parallel sample

is heated by a short light or laser pulse.

The temperature rise on the rear surface is

measured versus time using an IR detector.

The sample has been stabilized at the desired

temperature, the laser fired several times over a span

of a few minutes and the necessary data is recorded

for each laser shot. The laser beam energy strikes and is absorbed by the front surface of the sample,

causing a heat pulse to travel through the samples thickness. The resulting sample temperature rise is

fairly small, ranging from 0.5 to 2 C. The temperature rise is amplified and recorded.

• www.netzsch.com Thermal Diffusivity and Thermal Conductivity by LFA 11 11

Heat Transfer LFA Method

11

2/1

2

1337.0t

da

pcmT

1max

TTcTaT p

• www.netzsch.com

Heat Transfer: LFA Method

Polymer (slow) Metal (average) Graphite (fast)

Half-times

Thermal Diffusivity and Thermal Conductivity by LFA

• www.netzsch.com Thermal Diffusivity and Thermal Conductivity by LFA 13

Agenda

1. Heat Transfer - Basics

2. LFA - Method

3. LFA - Instrumentation

4. Application Examples

5. Summary

• www.netzsch.com

Flash Technique Introduction Netzsch LFA Systems for almost all application ranges

14

LFA 457 MicroFlash

-125C to 1100C

Sample changer for 3

samples

Thermal Diffusivity and Thermal Conductivity by LFA

LFA 467 HyperFlash

-100C to 500C

Sample changer for 16

samples

ZoomOptics - IR detector

Fastest data acquisition

LFA 427

-120C to 2800C

• www.netzsch.com

NETZSCH LFA 467 HyperFlash

Table-top instrument

Works with a high power Xenon-Flash

lamp

Temperature range: -100 to 500C

Integrated sample changer for

16 samples

Different cooling options

ZoomOptics for optimized field of view

• www.netzsch.com

NETZSCH LFA 467 HyperFlash ZoomOptics

No Zoom Optics Distortion from Aperture

Field of view is fixed, large enough to cover big diameter

samples.

Testing smaller diameter samples, apertures are used

minimizing the influence of the surroundings.

Significant distortion of the thermal curve: detector not

only senses the temperature rise of the sample, but also any

fluctuations from the aperture.

Thermal curve shows either a continuously increasing

trend or an extended leveling-off period.

Distortion from Aperture

• www.netzsch.com

NETZSCH LFA 467 HyperFlash ZoomOptics

Zoom Optics No Distortion from Aperture

IR signal originates solely from the sample surface

Large and small samples can be tested with an

optimal sensing area.

No contributions from the aperture

Thermal curve conforms to the theoretical model, yielding correct diffusivity values.

No Distortion from Aperture

• www.netzsch.com

NETZSCH LFA 467 HyperFlash

High Sample Throughput

Highest Sample Throughput

High Efficiency

16 Pyroceram samples (2.5

mm thick, 12.7 mm)

Thermal diffusivity shows a

deviation of 2% from

literature data.

Optimum position for each of

the 16 samples in the

furnace over the entire

temperature range.

Reduced measurement time

High throughput possible

without operators

intervention

• www.netzsch.com

NETZSCH LFA 467 HyperFlash

Thin and High Conductive Materials

Thin and High ConductiveCopper Copper samples with different thicknesses from 3.0 mm to 0.25 mm.

Measurements confirm that even very thin samples can be tested with very high accuracy.

Sample preparation and thickness determination have to be carefully considered when measuring thin samples. Especially graphite coating can lead to lower thermal diffusivity values.

0,1 1 10

0

10

90

100

110

120

130

Th

erm

al d

iffu

sivi

ty [m

m/

s]

Sample Thickness [mm]

LFA467

Literature

• www.netzsch.com

NETZSCH LFA 457 MicroFlash

Table-top unit with laser

Temperature range: -125 to 1100 C

(with two furnaces)

Integrated sample changer for 3 samples

• www.netzsch.com

Vertical system

Two exchangeable furnaces

-125 500C

RT 1100C

Vacuum-tight (1 Pa)

Laser pulse length ~ 0.33 ms

LFA 457 MicroFlash Design

• www.netzsch.com

LFA 457 MicroFlash

Sample Changer

Multiple Sample Arrangement12.7 mm dia. and 10.0 mm square

Single Sample Arrangement25.4 mm dia.

• www.netzsch.com

Standard Application Stainless Steel

0.40

0.45

0.50

0.55

0.60

0.65

Sp

ecific

He

at / (J

/(g

*K)

0 100 200 300 400 500 600 700 800 Temperature / C

2

3

4

5

6

Th

erm

al D

iffu

siv

ity / m

m/

s

Thermal Diffusivity

Specific Heat

DSC 404 Test

SRM 1461 - Stainless Steel

• www.netzsch.com

Application Filled Rubber

-125 -100 -75 -50 -25 0 25 50 75 100

Temperature / C

0.0

0.1

0.2

0.3

0.4

Therm

al D

iffusi

vity

/ m

m/

s

Sample: Filled NR/BR

Thickness: 1.512 mm

Width: 12.70 mm

0.0

0.1

0.2

0.3

0.4

0.5

Therm

al C

onduct

ivity

/ W

/(m

*K)

0.0

Recommended